"Nanoscale Zippers" in Gd5(SixGe1-x)4: Symmetry and Chemical Influences on the Nanoscale Zipping Action
Wonyoung Choe; A. O. Pecharsky; Michael Wörle; Gordon J. Miller; Inorganic Chemistry 42 (2003) 8223–8229; doi:10.1021/ic034941z

data_4312727
_publ_section_title
;
 "Nanoscale Zippers" in Gd5(SixGe1-x)4: Symmetry and Chemical Influences
 on the Nanoscale Zipping Action
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              8223
_journal_page_last               8229
_journal_paper_doi               10.1021/ic034941z
_journal_volume                  42
_journal_year                    2003
_chemical_formula_sum            'Gd6.67 Ge3.33 Si2'
_chemical_formula_weight         1346.48
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            3
_cell_length_a                   7.6652(12)
_cell_length_b                   14.809(2)
_cell_length_c                   7.7695(12)
_cell_measurement_temperature    293(2)
_cell_volume                     881.9(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.938
_diffrn_measured_fraction_theta_max 0.938
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0978
_diffrn_reflns_av_sigmaI/netI    0.0554
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            6358
_diffrn_reflns_theta_full        27.73
_diffrn_reflns_theta_max         27.73
_diffrn_reflns_theta_min         2.75
_exptl_absorpt_coefficient_mu    45.542
_exptl_crystal_density_diffrn    7.605
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1684
_refine_diff_density_max         3.467
_refine_diff_density_min         -3.196
_refine_diff_density_rms         0.731
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.811
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     49
_refine_ls_number_reflns         1004
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.811
_refine_ls_R_factor_all          0.0540
_refine_ls_R_factor_gt           0.0421
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1000P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1064
_refine_ls_wR_factor_ref         0.1128
_reflns_number_gt                828
_reflns_number_total             1004
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic034941zsi20030808_090521.cif
_cod_data_source_block           mil84d_2
_cod_original_cell_volume        882.0(2)
_cod_database_code               4312727